Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our User Agreement and Privacy Policy.

Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our Privacy Policy and User Agreement for details.

Like this document? Why not share!

896 views

Published on

No Downloads

Total views

896

On SlideShare

0

From Embeds

0

Number of Embeds

73

Shares

0

Downloads

0

Comments

0

Likes

2

No embeds

No notes for slide

- 1. Chapter 2 Anisotropic Elastic Solids Properties of composite materials and their constituents often depend on both position and direction in a ﬁxed system of coordinates. In the terminology of solid mechanics, such materials are heterogeneous and anisotropic. This chapter is concerned with the directional dependence, deﬁned by certain material symmetry elements, and reﬂected in eight distinct forms of the stiffness and compliance matrices of elastic solids. Such materials include, for example, reinforcing ﬁbers, particles and their coatings, or ﬁbrous composites and laminates represented on the macroscale by homogenized solids with equivalent or effective elastic moduli. Identiﬁcation of the positions of zero-valued coefﬁcients, and of any connections between nonzero coefﬁcients in those matrices is of particular interest. Different classes of crystals exhibit a much larger range of symmetries, derived from spatial arrangement of their lattices. Broader expositions of these topics can be found in several books, such as Love (1944), Lekhnitskii (1950), Green and Atkins (1960), Nye (1957, 1985), Hearmon (1961), Ting (1996), and Cowin and Doty (2007). 2.1 Elastic Strain Energy Density The elastic strain energy stored in a unit volume of a homogeneous elastic material that is subjected to a certain uniform local strain state ".c/ is deﬁned by a scalar quantity W .".c/ /, the strain energy density. Any deformation leading to another strain state, that starts at and is then reversed to ".c/ , has no effect on the magnitude of W .".c/ /, hence the energy density is independent of the deformation path followed to reach the current strain. The energy accumulated in the unit volume is W D ".c/ Z 0 ijd"ij D ".c/ Z 0 Lijkl"kld"ij (2.1.1) G.J. Dvorak, Micromechanics of Composite Materials, Solid Mechanics and Its Applications 186, DOI 10.1007/978-94-007-4101-0 2, © Springer ScienceCBusiness Media B.V. 2013 11
- 2. 12 2 Anisotropic Elastic Solids This integral is path independent if the integrand is the total differential dW D @W @"ij d"ij D Lijkl"kld"ij D 1 2 d.Lijkl"kl"ij/ (2.1.2) where d.Lijkl"kl"ij/ D Lijkl."kld"ij C "ijd"kl/. The second derivative must be independent of the order of differentiation, hence the integrand @2 W @"kl@"ij D @2 W @"ij@"kl ) Lijkl D Lklij (2.1.3) as anticipated by (1.1.7). The argument leading to (2.1.3) can also be utilized to show independence of the complementary energy on the stress path, and diagonal symmetry of the compliance matrix Mijkl D Mklij . Following the contraction (1.1.8) to (6 6) matrices, both L˛ˇ and M˛ˇ.˛; ˇ D 1; 2; : : : 6/ are real and diagonally symmetric, with at most 21 independent coefﬁcients. Integration of (2.1.2) provides 2W D Lijkl"ij"kl D Mijkl ij kl D ij"ij > 0 2W D L˛ˇ"˛"ˇ D M˛ˇ ˛ ˇ D "ˇ ˇ > 0 ) (2.1.4) where i; j; : : : D 1; 2; 3, ˛; ˇ, : : : D 1, 2, : : : 6. Moreover, "˛; "ˇ are the engineering strain components and the stiffness and compliance matrices LEG ! L˛ˇ; MEG ! M˛ˇ. The strain energy density W is a positive deﬁnite quadratic form and both L˛ˇ and M˛ˇ are positive deﬁnite matrices, with real, positive eigenvalues. Decomposition of the stress and strain tensors according to (1.1.14), enables writing of the strain energy density as a sum of distortional and dilatational parts W D 1 2 ij"ij D 1 2 Â 1 3 kkıij C sij Ã Â 1 3 "kkıij C eij Ã D 1 6 kk"kk C 1 2 sijeij (2.1.5) where sijıij D eijıij D 0I ıijıij D 3: In the absence of a speciﬁc constitutive relation that evaluates the coefﬁcients of L˛ˇ or M˛ˇ, this form of W is valid for any material symmetry. Transcription of the energy function into the contracted tensorial and engineering (EG) notations is facilitated by expanding the product ij"ij in (2.1.5) 2W D ij"ij D 11"11 C 22"22 C 33"33 C 2 12"12 C 2 23"23 C 2 31"31 (2.1.6)
- 3. 2.1 Elastic Strain Energy Density 13 In the two notations, this result is provided by the products derived using (1.1.12) 2W D "ij ij ! "T D T " D "T EG D T "EG 2W D T "EG D "T EGLEG"EG D "T L"EG D "T L " ) (2.1.7) This shows that the product "T EGLEG"EG of engineering strain and stiffness matrices provides the correct magnitude of the strain energy, to be used in Chap. 5. However, the following invariants transcribe as sijsij D s2 11 C s2 22 C s2 33 C 2.s2 23 C s2 31 C s2 12/ ! sT s (2.1.8) and eijeij D e2 11 C e2 22 C e2 33 C 2.e2 23 C e2 31 C e2 12/ ! eT e D eT EG 1 eEG (2.1.9) The results indicate that transcription of tensorial expressions to matrix form needs to be performed with care. Apart from the diagonal symmetry derived in (2.1.3), the structure of the elastic stiffness and compliance matrices depends on material symmetry, deﬁned by reﬂection or symmetry planes and axes of rotational symmetry in Sect. 2.2. For each material symmetry, the inequalities (2.1.4) impose certain restrictions or bounds on the values of stiffness and compliance coefﬁcients. Ting (1996) indicates that these restrictions provide more stringent limitations on elastic constants than those which ensure that the differential equations governing elastostatic problems are completely elliptic. Within their particular limits, the elastic moduli may exhibit signiﬁcant changes and assume extreme values, as discussed in Sect. 2.5. Nye (1985), among others, shows examples of directional dependence of elastic moduli of certain crystals. The necessary and sufﬁcient conditions for positive deﬁniteness of stiffness and compliance matrices require that all principal minors of L˛ˇ or M˛ˇ be positive. The minors are determinants of the ﬁve principal submatrices, generated by deleting same numbered rows and columns; they include the determinants L˛ˇ and M˛ˇ . This guarantees that all diagonal terms of L˛ˇ or M˛ˇ, as well as all eigenvalues of these matrices are positive. As a positive deﬁnite and symmetric quadratic form, the strain energy density can also be written as a polynomial in the strain components, arranged as strain invariants consistent with the groups of transformations describing a particular crystal class. A complete list of the invariants appears in Green and Atkins (1960). Several different invariants of the anisotropic elasticity tensor with respect to arbitrary orthogonal transformations are discussed, for example, by Spencer (1971), Ting (1987), Ahmad (2002) and Ting and He (2006). Evaluation of the effect of material symmetry on the structure of the stiffness and compliance matrices is facilitated by reference to the expanded form (2.1.4)
- 4. 14 2 Anisotropic Elastic Solids of the strain energy density W ."˛ˇ/. Recall from (2.1.7) that 2W D "T EGLEG"EG, hence the expanded form is written using engineering strains "EG ! "˛ from (1.1.11) and LEG ! L˛ˇ W "˛ˇ D L11"2 1=2 CL12"1"2 CL13"1"3 CL14"1"4 CL15"1"5 CL16"1"6 CL22"2 2=2 CL23"2"3 CL24"2"4 CL25"2"5 CL26"2"6 CL33"2 3=2 CL34"3"4 CL35"3"5 CL36"3"6 CL44"2 4=2 CL45"4"5 CL46"4"6 CL55"2 5=2 CL56"5"6 CL66"2 6=2 9 >>>>>>>= >>>>>>>; (2.1.10) Speciﬁc symmetry elements are introduced by certain coordinate transformations which are required to preserve invariance of W ."˛ˇ/. A strain component that changes its sign as a result of the transformation may change the expanded form of W . To prevent that, the stiffness coefﬁcients appearing in the affected terms of W are made equal to zero. For example, if a particular coordinate transformation induces a sign change in the strain "5, from C"5 to "5, then L15 D L25 D L35 D L45 D L56 D 0 in the stiffness matrix of the solid deﬁned by this transformation. Additional reductions follow from connections established between nonzero coefﬁcients. In this manner, accumulation of symmetry elements reduces the number of independent elastic moduli from the maximum of 21 to the minimum of 2, in isotropic solids. Of course, identical coefﬁcient reductions apply to both LEG and L, and also to MEG and M: 2.2 Material Symmetries 2.2.1 Elements of Material Symmetry Early studies of material symmetry were inspired by observed properties of crystals. Voigt (1910) identiﬁed 32 crystal classes, among eight basic symmetry groups of transformations that preserve a particular form of W . A systematic classiﬁcation of crystal symmetries and complete groups of transformations for each crystal class are described in Green and Atkins (1960), following the formalism developed by Smith and Rivlin (1958). For each crystal class, their results also include representations of W by polynomials, in terms of sets of strain component invariants which form a polynomial basis for each transformation group. The related stress invariants have been used in deﬁnitions of assumed yield or failure surfaces of anisotropic solids (Hill 1948; Mulhern et al. 1967, 1969; Spencer 1972; Tsai and Wu 1971). A systematic formulation of general principles, and of equilibrium, transport and optical properties of crystals can be found in Nye (1957, 1985).
- 5. 2.2 Material Symmetries 15 More recent studies, initiated by Cowin and Mehrabadi (1987, 1989) show that the eight basic symmetries can be deﬁned by the number of planes of symmetry that each one admits, without reliance on the groups of transformations or crystallography. These results also allow determination of material symmetry of materials with initially unknown microstructures. For a comprehensive review, see Cowin and Mehrabadi (1995), Cowin and Doty (2007). Chadwick et al. (2001) reconcile the symmetry groups and symmetry planes approaches and show their equivalence. Ting (1996, 2003) provides a concise exposition of the number and orientation of symmetry planes for each of the eight symmetries. Here we make contact with a subset of these results, and emphasize symmetry elements that can be identiﬁed by inspection of the microstructure of composite materials and laminates. Each symmetry element will be deﬁned by a speciﬁc form of the matrix aij of directional cosines in (2.2.1) below. Applying this aij matrix yields transformed strain components, some of which may change values of certain terms of the strain energy density function W displayed in (2.1.10). As already mentioned, invariance of W under each such transformation is preserved by letting the stiffness coefﬁcients of L˛ˇ be equal to zero, in the terms changed by the transformation. The strain energy density W corresponding to a particular com- bination of material symmetry elements is generated by application of successive transformations, one for each of the speciﬁed symmetry elements. We consider only the effect of symmetry on the stiffness and compliance matrices, or on fourth order tensors that relate two second order tensors. Tensors deﬁning transport and other properties experience different material symmetry effects, described by (Nye 1957, 1985), and with speciﬁc applications later. Coordinate transformations consistent with the Euclidean space are translations, rotations and reﬂections, described by x0 i D x0 i C aijxj aij D cos.x0 i ; xj / i; j D 1; 2; 3 (2.2.1) where x0 i 2 V is the translation vector, and the aij is an orthogonal matrix of directional cosines which describes the reﬂection and rotation parts of the transformation. Material symmetry in the Euclidean space requires the strain energy density W in (2.1.10) to remain invariant under coordinate transformations of both strain and stress components, implied by reﬂection or symmetry planes and axes of rotational symmetry. W ."0 ˛ˇ/ D W ."˛ˇ/ W . 0 ˛ˇ/ D W . ˛ˇ/ (2.2.2) Translational invariance assures homogeneity, or the same symmetry everywhere in a given material volume; it has no effect on material symmetry itself. Material symmetry elements include, as appropriate, the three coordinate planes and one or more planes of symmetry, or reﬂection planes aligned with the x3 axis, each deﬁned by a unit normal vector ni that contains an angle ™ with the
- 6. 16 2 Anisotropic Elastic Solids Fig. 2.1 Evolution of material symmetries by addition of planes and axes of symmetry x1 axis, measured counterclockwise, Fig. 2.1. Also, a vector mj is deﬁned in the plane itself. When such transformation is a reﬂection, the normal vector may reverse its direction, such that aijnj D ni , while the aijmj D mi . The corresponding matrix of directional cosines is aij D ıij 2ni nj (2.2.3) In particular, if the normal vector is ni D Œcos ™; sin ™; 0T , =2 < ™ 6 =2, then the reﬂection (2.2.3) is described by the transformation aij D 2 4 cos 2™ sin 2™ 0 sin 2™ cos 2™ 0 0 0 1 3 5 (2.2.4) Also included among symmetry elements are axes of rotational symmetry, each deﬁned by a unit axial vector and by the angle of rotation ™ D 2 =n; and called a n-th order or n-fold axis. For example, the transformation describing a rigid body rotation by an angle ™ about the x3 axis; measured counterclockwise from ™ D 0 at x2 D 0 is
- 7. 2.2 Material Symmetries 17 aij D 2 4 cos ™ sin ™ 0 sin ™ cos ™ 0 0 0 1 3 5 (2.2.5) Each of the eight material symmetries can be described by one or more reﬂection planes and/or axes of rotational symmetry. In all anisotropic materials, both the strain energy and stiffness are invariant under central inversion, denoted by C and deﬁned by selecting aij D ıij, as well as under identity or I3 transformation aij D ıij. The identity aaT D aT a D I3 ) aT D a 1 shows that a material symmetry deﬁned by an orthogonal (3 3) matrix a is also deﬁned by aT D a 1 . The implication is that a material symmetric with respect to rotation by a certain angle ™ remains symmetric when rotated by ™. Additional symmetry elements, such as glide planes, and n-fold screw and inversion axes are used in crystal physics (Nye 1957, 1985). Figure 2.1, shows schematically the eight material symmetries, with their symmetry elements and interconnections, described in the following paragraphs. In the triclinic material at the upper left, there are no symmetry planes or axes, while in the isotropic material at the lower right, any plane and axis is an element of symmetry. 2.2.2 Triclinic Materials No reﬂection planes or axes of rotational symmetry are prescribed to impose restrictions on the structure of the stiffness matrix, which remains fully populated by 21 independent coefﬁcients L˛ˇ. Therefore, triclinic solids are symmetric only with respect central inversion C, allowing for transformations I3 and I3, C, which are shared by all material symmetries. In addition to the triclinic crystals, the fully populated matrices frequently appear in constitutive relations of elastic-plastic and other inelastic materials, where they may represent an instantaneous tangential or secant stiffness at a particular point of the deformation path. Cowin and Mehrabadi (1995, §10), indicate that a coordinate system can be selected such that three components of L˛ˇ of the triclinic system become equal to zero, reducing the number of nonzero coefﬁcients to 18. 2.2.3 Monoclinic Materials A single plane of material symmetry is introduced, typically selected as one of the three coordinate planes. For example, reﬂection about the x1x2-plane at x3 D 0 is described by
- 8. 18 2 Anisotropic Elastic Solids Table 2.1 Stiffness matrices of triclinic, monoclinic and orthotropic solids 2 6 6 6 6 6 6 4 3 7 7 7 7 7 7 5 2 6 6 6 6 6 6 4 0 0 0 0 0 0 0 0 3 7 7 7 7 7 7 5 2 6 6 6 6 6 6 4 0 0 0 0 0 0 0 0 3 7 7 7 7 7 7 5 2 6 6 6 6 6 6 4 0 0 0 0 0 0 0 0 0 0 0 0 3 7 7 7 7 7 7 5 Triclinic Monoclinic (symm. plane x3 D 0) Monoclinic (symm. plane x1 D 0) (Orthotropic, Rhombic) m D 21 m D 13 m D 13 m D 9 aij D cos x0 i ; xj D 2 4 1 0 0 0 1 0 0 0 1 3 5 (2.2.6) which provides transformed strains "0 ˛ "0 1 D "1 "0 2 D "2 "0 3 D "3 "0 4 D "4 "0 5 D "5 "0 6 D "6 (2.2.7) Invariance of W in (2.1.10), with respect to the transformation (2.2.6), requires the terms affected by the above strain sign changes to vanish. That is enforced by setting L14 D L15 D L24 D L25 D L34 D L35 D L46 D L56 D 0 (2.2.8) which reduces the number of stiffness coefﬁcients from 21 to 13. The stiffness matrix for reﬂection about x1x2 plane appears in Table 2.1, where each bullet stands for a different stiffness coefﬁcient. When substituted into the matrix form of the constitutive relation (1.1.21), the nonzero coefﬁcients in the upper right (3 3) partition, and the off-diagonal coefﬁcients L45 or L56 in the lower right partition of these matrices cause coupling between normal strains and shear stresses, and between different shear strain and stress components. The letter m denotes the number of independent stiffness and compliance coefﬁcients in the respective matrices. Cowin and Mehrabadi (1995, §10) show that certain restricted rotations about the normal to the plane of symmetry provide further reduction of the non-zero coefﬁcients from 13 to 12. If the x2x3 plane of symmetry is chosen at x1 D 0, then permutation of subscripts in (2.2.8) yields the vanishing stiffness and compliance coefﬁcients L15 D L16 D L25 D L26 D L35 D L36 D L45 D L46 D 0 (2.2.9)
- 9. 2.2 Material Symmetries 19 Finally, for the x1x3 plane at x2 D 0 L14 D L16 D L24 D L26 D L34 D L36 D L45 D L56 D 0 (2.2.10) Table 2.1 displays the stiffness matrices complying with (2.2.8) and (2.2.9). Monoclinic symmetry applies, for example, to a homogenized unidirectional ﬁbrous ply in the overall coordinate system of a laminated plate, when the ﬁbers contain an arbitrary angle with the 0ı direction of the laminate. Although the ply may have a higher, transversely isotropic symmetry in the local coordinates of the ply, in the overall system it has only reﬂective symmetry about any plane parallel to its mid-plane. 2.2.4 Orthotropic Materials Together with rhombic and orthorombic crystals, orthotropic solids have three mutually perpendicular planes of reﬂective symmetry, with normals in the directions of the coordinate axes. These symmetry planes include those with ™ D 0; =2 in Fig. 2.1. Therefore, the form of W is found by superimposing (2.2.8) with reﬂections about the x2x3 and x1x3 planes, which are indicated in (2.2.9) and (2.2.10), respectively. It can be veriﬁed by inspection of (2.2.8), (2.2.9), (2.2.10) that using only two of the three symmetry planes yields the same zero-valued stiffness coefﬁcients. However, the planes are not exchangeable, since material properties remain distinct in the three coordinate directions. The number of independent moduli is reduced to a total of nine, with six on the main diagonal and L12; L13; L23 in the upper left (3 3) partition; Table 2.1. No coupling terms remain in the upper or lower right partition. The compliance matrix has the same structure, with M˛ˇ coefﬁcients replacing the L˛ˇ. The zero-valued coefﬁcients are L˛4 D L˛5 D L˛6 D 0 for ˛ D 1; 2; 3 and L45 D L46 D L56 D 0 (2.2.11) Layered plane materials, such as composite laminates and plywood often exhibit orthotropic symmetry on the macroscale, in terms of effective or overall properties derived by homogenization of the material volume. However, on the more reﬁned scale that recognizes individual layers or plies, these materials do not satisfy, in the direction normal to the interfaces, the translational invariance condition (2.2.1) that embodies the homogeneity requirement.
- 10. 20 2 Anisotropic Elastic Solids Table 2.2 Stiffness matrices of trigonal and tetragonal solids 2 6 6 6 6 6 6 4 L11 L12 L13 L14 0 0 L11 L13 L14 0 0 L33 0 0 0 L44 0 0 L44 L14 .L11 L12/=2 3 7 7 7 7 7 7 5 2 6 6 6 6 6 6 4 L11 L12 L13 0 0 0 L11 L13 0 0 0 L33 0 0 0 L44 0 0 L44 0 L66 3 7 7 7 7 7 7 5 Trigonal, axis rot.symm: x3 Tetragonal, axis rot. symm: x3 m D 6 m D 6 2.2.5 Trigonal and Tetragonal Materials In contrast to the orthotropic symmetry, these materials are deﬁned by prescribing certain equivalent planes of elastic symmetry, that require retention of material properties after exchange of the equivalent symmetry planes. Such exchange may be accomplished by rotation about a ﬁxed axis of symmetry. For example, a rigid body rotation by an angle ™ about the x3 axis; measured ccw from ™ D 0 at x2 D 0 as indicated by (2.2.5). A trigonal material admits rigid body rotation about a 3-fold axis x3, such that W in (2.1.10) remains invariant at ™ D 0; ˙ =3. This deﬁnes three equivalent planes, all aligned with x3 and separated by 60ı angles. The x1x2 plane is not a reﬂection plane. The principal diagonal of the stiffness matrix has only three inde- pendent coefﬁcients, but coupling coefﬁcients L14 D L24 D L56 are still present (Table 2.2). L11 DL22 L44 D L55 2L66 D .L11 L12/ L13 D L23 L14 D L24 D L56 L˛5 D L˛6 D 0 for ˛ D 1; 2; 3; 4 9 >>= >>; (2.2.12) A tetragonal material, has the x1x2 plane of reﬂection, and it admits a rigid body rotation about a 4-fold axis x3, with invariance of W preserved at ™ D 0; ˙ =4; =2: Therefore, the planes aligned with x3 are separated by 45ı angles, and they are equivalent or exchangeable planes of symmetry. To keep the strain energy (2.1.10) invariant under the transformations indicated by these symmetries, the following stiffness coefﬁcients are connected or set equal to zero L11 D L22 L44 D L55 L13 D L23 L˛4 D L˛5 D L˛6 D 0 for ˛ D 1; 2; 3 L45 D L46 D L56 D 0 ) (2.2.13) Both trigonal and tetragonal materials have m D 6 nonzero stiffness or compli- ance coefﬁcients, which are not identically positioned or related.
- 11. 2.2 Material Symmetries 21 2.2.6 Transversely Isotropic or Hexagonal Materials These materials have two symmetry elements, one plane that may be selected as the x1x2 plane in Fig. 2.1, and perpendicular to that plane, an axis or rotational symmetry x3 about any angle ™. In the x1x2 plane of symmetry, the material is isotropic, with properties independent of direction, so that all planes containing the x3 axis are also planes of symmetry. The matrix of directional cosines that describes rotation around x3 by an angle ™, measured counter-clockwise from x1 to x0 1; is shown by (2.2.5). The strains "0 ij D aikajl "kl are "0 11 D "11cos2 ™ C "22sin2 ™ 2"12 sin ™ cos ™ "0 22 D "11sin2 ™ C "22cos2 ™ C 2"12 sin ™ cos ™ "0 33 D "33 "0 13 D "13 cos ™ "23 sin ™ "0 23 D "13 sin ™ C "23 cos ™ "0 12 D ."11 "22/ sin ™ cos ™ "12 sin2 ™ cos2 ™ 9 >>>>>= >>>>>; (2.2.14) It can be veriﬁed that the following ﬁve strain invariants associated with transverse isotropy about x3 D 0 are independent of the transformation (2.2.5). The strain energy W can be written as a polynomial in these invariants "0 33 D "33 "0 11 C "0 22 D "11 C "22 "0 11"0 22 "0 12 2 D "11"22 "2 12 "0 13 2 C "0 23 2 D "2 13 C "2 23 ˇ ˇ"0 ij ˇ ˇ D ˇ ˇ"ij ˇ ˇ 9 >>>= >>>; (2.2.15) Coefﬁcients of the stiffness or compliance matrix are connected as those of the trigonal system in (2.2.12), but by introduction of the x1x2 plane of symmetry, they are further reduced to L14 D L15 D L56 D 0: That leaves ﬁve independent constants and zero coupling terms, as also shown in Table 2.3. Moreover, the constants need to satisfy (2.1.4) which requires the strain energy to be a positive deﬁnite quadratic form. This yields the connections (Nye 1985) L11 D L22 > jL12j L44 D L55 > 0 2L66 D .L11 L12/ L13 D L23 L14 D L15 D L56 D 0 .L11 C L12/L33 > 2L2 13 L˛5 D L˛6 D 0 for ˛ D 1; 2; 3; 4 9 >>= >>; (2.2.16) The same results follow for hexagonal or higher symmetry, when ™ D =n and n > 3:
- 12. 22 2 Anisotropic Elastic Solids Table 2.3 Stiffness matrices of transversely isotropic solids 2 6 6 6 6 6 6 4 L11 L12 L13 0 0 0 L11 L13 0 0 0 L33 0 0 0 L44 0 0 L44 0 .L11 L12/=2 3 7 7 7 7 7 7 5 2 6 6 6 6 6 6 4 L11 L12 L12 0 0 0 L22 L23 0 0 0 L22 0 0 0 .L22 L23/=2 0 0 L55 0 L55 3 7 7 7 7 7 7 5 Axis of rotational symmetry: x3 Axis of rotational symmetry: x1 m D 5 m D 5 Materials reinforced by ﬁbers aligned in a single direction and randomly distributed in the transverse plane are regarded as transversely isotropic. A more extensive description of this symmetry, in notations commonly applied to unidirec- tional composites, appears in Sect. 2.3. 2.2.7 Cubic Materials Nine planes of elastic symmetry are prescribed, arranged in sets of three and derived from the tetragonal symmetry. Three of the nine planes are perpendicular to the coordinate axes, and are interchangeable. Six planes have normals that contain an angle =4 with the coordinate axes. Only three independent constants remain, and they must satisfy (2.1.4). This yields the following connections (Nye 1985) L11 DL22 D L33 > j L12j L12 D L13 D L23 L44 DL55 D L66 > 0 L11 C 2L12 > 0 ) (2.2.17) The remaining 12 coefﬁcients are all equal to zero. Many metals and ceramics crystallize in either tetragonal, or face or body-centered cubic system. Analytical studies often prefer to employ the bulk modulus Ä and two shear moduli and 0 which Zener (1948) identiﬁes by means of the connections (Walpole 1981, 1985a) Ä D 1 3 .L11 C 2L12/ D 1 2 .L11 L12/ 0 D L44 (2.2.18) In fact, and 0 are two extreme shear moduli that bound every other shear modulus of the crystal. In an isotropic solid, they coincide as the unique shear modulus. The extent to which their ratio 0 = differs from unity is a measure of anisotropy. In general, 0 is larger than in most actual cubic crystals. All three moduli Ä, and 0 are necessarily positive in accordance with the positive deﬁniteness of the strain energy in (2.1.4).
- 13. 2.2 Material Symmetries 23 The nonzero coefﬁcients of the compliance matrix in engineering notation can be written as M11 DM22 D M33 D 1 9Ä C 1 3 M12 D M13 D M23 D 1 9Ä 1 6 M44 D M55 D M66 D 1 0 9 >>= >>; (2.2.19) 2.2.8 Isotropic Materials At least three perpendicular axes of rotational symmetry about any angle are available. Any plane is a plane of symmetry, and invariance of the strain energy W is preserved under any orthogonal transformation of the coordinates. In addition to the connections (2.2.17), the shear moduli are equal, which reduces the number of independent moduli from three to two. L11 D L22 D L33 L12 D L13 D L23 L44 D L55 D L66 D 1 2 .L11 L12/ M11 D M22 D M33 M12 D M13 D M23 M44 D M55 D M66 D 2.M11 M12/ 9 = ; (2.2.20) The stiffness matrix of isotropic solids in the engineering notation is LEGD E .1 C /.1 2 / 2 6 6 6 6 6 6 6 4 1 0 0 0 1 0 0 0 1 0 0 0 .1 2 /=2 0 0 .1 2 /=2 0 .1 2 /=2 3 7 7 7 7 7 7 7 5 (2.2.21) The contracted tensorial stiffness matrix L in (1.1.22), written with bulk modulus K, shear modulus G has the nonzero coefﬁcients L11 DL22 D L33 D .3K C 4G/=3 L12 DL13 D L23 D L21 D L31 D L32 D .3K 2G/=3 L44 DL55 D L66 D 2G 9 >>= >>; (2.2.22) The matrix LEG is usually written using the Lam´e constants ; , with L11 D C2 ; L12 D and L44 D , repeated as indicated above. Relations between these
- 14. 24 2 Anisotropic Elastic Solids and the Young’s modulus E, bulk modulus K, shear modulus G, and the Poisson’s ratio are D E .1 C /.1 2 / D K 2 3 G E D 9KG 3K C G D G D E 2.1 C / K D E 3.1 2v/ 9 >>= >>; (2.2.22a) Both LEG and L appear in the constitutive relation ˛ D L˛ˇ"ˇ; .˛; ˇ D 1; 2; : : : 6/ where the stress and engineering or tensorial strain vectors are deﬁned by (1.1.9)–(1.1.11). The compliance matrix has a similar structure, with MEG written as M11 DM22 D M33 D 1=E M12 D M13 D M23 D =E M44 D M55 D M66 D 1=G D 1= ) (2.2.23) In the contracted tensorial component M matrix, M44 D M55 D M66 D 1=2G D 1=2 . For isotropic solids with elastic moduli K and G, the strain energy function (2.1.5) is evaluated using kk D 3K"kk; sij D 2Geij. The result is 2W D 1 9K . kk/2 C 1 G J2 D K."kk/2 C 2Geijeij (2.2.24) where J2 D sijsij=2 is the second invariant of the stress deviator tensor. Since each of the two terms has to be positive deﬁnite, the moduli must satisfy G > 0; K > 0. This also implies that E D 9KG 3K C G ) E > 0 D 3K 2G 2.3K C G/ ) 1 < < 1 2 (2.2.25) In materials regarded as rigid, all moduli become inﬁnite. The Poisson’s ratio approaches the low limit ! 1 for G ! 1 and ﬁnite K. The high limit ! 0:5 is observed in incompressible materials, where K ! 1 and G remains bounded. For example, 0:45 0:49 in soft rubbers and biological tissues, 0.33 in aluminum, 0.29 in steel, 0.1–0.4 or negative in certain polymer foams and nearly zero in cork (Lakes 1987). Isotropic material symmetry applies to metals, ceramics and certain polymers, at scales exceeding the typical grain size by at least one order of magnitude, where translational invariance in (2.2.1) can be accepted. Applications at more reﬁned scales are justiﬁed by lack of data or simplicity of modeling. Different deﬁnitions of material symmetry and isotropy in particular have been developed for materials with cellular and other heterogeneous microstructures.
- 15. 2.2 Material Symmetries 25 For example, Christensen (1987) shows that only six axes of ﬁve-fold symmetry associated with the pentagonal dodecahedron and the icosahedron are sufﬁcient for isotropy of cellular and low density materials which transmit load by axial deformation of micro-struts arranged in a space network. The corresponding ﬁber composite is isotropic if the ﬁbers take at least the six speciﬁc directions in three- dimensional space. Budiansky and Kimmel (1987) present a different derivation of isotropy for the macroscopic moduli of lung tissue modeled by a pin-jointed truss, again in the shape of the regular pentagonal dodecahedron. 2.2.9 Decomposition of Isotropic Tensors and Matrices As shown in (1.1.16), the isotropic fourth-orderidentity tensor is a sum of two fourth rank tensors, Iijkl D Jijkl C Kijkl. Inner products of these tensors show that they are isotropic and idempotent JijklJklmn D 1 9 ıijıklıklımn D 1 3 ıijımn D Jijmn KijklKklmn D IijklKklmn Jijkl.Iklmn Jklmn/ D Kijmn JijklKklmn D Jijkl.Iklmn Jklmn/ D 0 9 >>>>= >>>>; (2.2.26) Moreover, since ıklıkl D 3, Jijij D 1; Kijij D 5; Jiijj D 3; Kiijj D 0: These properties simplify evaluation of inner products of isotropic fourth rank tensors, such as stiffness and compliance tensors of isotropic solids, which both depend on at most two elastic moduli. The inner product then is Uijkl D u1Jijkl C u2Kijkl Vijkl D v1Jijkl C v2Kijkl UijklVlkmn D u1v1Jijmn C u2v2Kijmn U 1 ijkl D 1 u1 Jijkl C 1 u2 Kijkl UijklU 1 lkpq D Iijpq 9 >>>>>= >>>>>; (2.2.27) where us; vs; s D 1; 2; are positive scalars. It can be veriﬁed that the .6 6/ matrices representing the tensors in the contracted tensorial notation also exhibit the above properties J D JJ D JT K D KK D KT KJ D JK D 0 J C K D I U D u1J C u2K U 1 D 1 u1 J C 1 u2 K U U 1 D I 9 >= >; (2.2.28)
- 16. 26 2 Anisotropic Elastic Solids Application to the stiffness matrices (2.2.21) and (2.2.22), written in the con- tracted tensorial notation . ! 2G in L44; L55; L66/, with the bulk and shear moduli K and G, yields L D 3KJ C 2GK M D 1 3K J C 1 2G K LM D I (2.2.29) where the matrices J and K were evaluated in (1.1.19). The coefﬁcients Lij appear in (2.2.22). The multiplication table (2.2.28) can be used to show that substitution of the above stiffness L and of both and " from (1.1.18) into D L " in (1.1.21), yields the elastic constitutive relation in the form J D 3KJ" and K D 2GK", or kk D 3K"kk and sij D 2Geij. Walpole (1981, 1984) and Baerheim (1993) provide similar ‘spectral’ decom- positions, and multiplication tables analogous to (2.2.28), for anisotropic tensors. However, their relative complexity limits widespread applications. 2.2.10 Orientation Average of a Fourth-Order Tensor An isotropic fourth order tensor can also be created as an average of an anisotropic tensor Hijkl, taken over all orientations. Under any orthogonal transformation (1.1.1) of Hijkl, there are only two linear invariants, Hijij and Hiijj (Ting 1987, 1996). If Hijkl is represented by a .6 6/ matrix H , not necessarily symmetric and written in tensorial component notation, then the invariants are Hijij ! h1 C h3 Hiijj ! h1 C h2 h1 D .H11 C H22 C H33/ h3 D .H44 C H55 C H66/ h2 D .H12 C H13 C H21 C H23 C H31 C H32/ 9 >>= >>; (2.2.30) With reference to the ‘spectral’ decomposition (2.2.29), the orientation average of fH g has the form (Kr¨oner 1958) fH g D aJ C bK fH g 1 D 1 a J C 1 b K (2.2.31) The scalars a; b are a D 1 3 Hiijj b D 1 5 Hijij a (2.2.32) Evaluation of the nonzero coefﬁcients of the .6 6/ matrix fH˛ˇg D fH˛ˇgT shows that
- 17. 2.3 Transversely Isotropic Composite Materials 27 fHg11 D fHg22 D fHg33 D 1 15 .3h1 C h2 C 2h3/ fHg12 D fHg13 D fHg23 D 1 15 .h1 C 2h2 h3/ fHg44 D fHg55 D fHg66 D 1 15 .2h1 h2 C 3h3/ 9 >>>>>>= >>>>>>; (2.2.33) As an exercise, one may verify that these relations yield (2.2.31) for any H D aJ C bK. Orientation averages of anisotropic tensors are useful in modeling of polycrystals and composites consisting of randomly orientated grains or constituents. 2.3 Transversely Isotropic Composite Materials 2.3.1 Engineering and Hill’s Moduli Experimental measurements of elastic moduli of ﬁbrous plies are usually performed on thin plies in the x1x2 plane, or on thin-walled cylindrical tubes with ﬁbers aligned along the longitudinal x1-axis. Details of such experiments appear, for example, in Herakovich (1998), and Daniel and Ishai (2006). Table 2.4 describes deﬁnitions of the engineering moduli, in terms of the strains measured in thin plies, under loading by a single stress component that needs to be applied for their experimental determination. Fibers are assumed aligned along the longitudinal x1-axis. Transverse isotropy about x1 and diagonal symmetry of Mij also yield E22 D E33 G23 D E22 2.1 C 23/ 21 E22 D 12 E11 23 D 32 (2.3.1) Note that transverse shear modulus G23 D m depends on Poisson’s ratio 23, derived from the out-of-plane strain "33 caused by the stress 22. Values of the shear modulus are seldom included in ply property data, since reliable measurement of "33 requires very large specimen thicknesses relative to those of a typical ply (0.13– 0.23 mm). Table 2.4 Evaluation of engineering moduli of ﬁbrous plies Applied Measured Calculated 11 "11, "22 D "33 E11 D 11/"11, 12 D "22/"11 D 13 22 "11, "22, "33 E22 D 22/"22, 21 D "11/"22, 23 D "33/"22 12 "EG 12 G12 D 12=.2"EG 12 /
- 18. 28 2 Anisotropic Elastic Solids The engineering compliance matrix Mij and the constitutive relation of a ply material are, for xA Á x1 2 6 6 6 6 6 6 6 4 "11 "22 "33 2"23 2"31 2"12 3 7 7 7 7 7 7 7 5 D 2 6 6 6 6 6 6 6 4 1=E11 21=E22 21=E22 0 0 0 12=E11 1=E22 32=E22 0 0 0 12=E11 23=E22 1=E22 0 0 0 0 0 0 1=G23 0 0 0 0 0 0 1=G12 0 0 0 0 0 0 1=G12 3 7 7 7 7 7 7 7 5 2 6 6 6 6 6 6 6 4 11 22 33 23 31 12 3 7 7 7 7 7 7 7 5 (2.3.2) The stiffness matrix of transversely isotropic solids is simpliﬁed by deﬁning the coefﬁcients of Lij by Hill’s (1964) moduli k, l, n, m, p, written here for consistency with (2.3.2) with the axis of rotational symmetry xA Á x1, to yield 2 6 6 6 6 6 6 6 4 11 22 33 23 31 12 3 7 7 7 7 7 7 7 5 D 2 6 6 6 6 6 6 6 4 n l l 0 0 0 l k C m k m 0 0 0 l k m k C m 0 0 0 0 0 0 m 0 0 0 0 0 0 p 0 0 0 0 0 0 p 3 7 7 7 7 7 7 7 5 2 6 6 6 6 6 6 6 4 "11 "22 "33 2"23 2"31 2"12 3 7 7 7 7 7 7 7 5 (2.3.3) where k D Œ2.1 23/=E22 4 2 12=E11 1 l D 2k 12 n D E11 C 4k 2 12 D E11 C l2 =k m D G23 p D G21 9 = ; (2.3.4) E11 D n l2 =k 12 D l=2k 21 D E22 12=E11 E22 D E33 D 4m.kn l2 / n.k C m/ l2 23 D 32 D n.k m/ l2 n.k C m/ l2 9 >= >; (2.3.5) Here, k is the transverse bulk modulus, or plane strain bulk modulus for lateral dilatation without axial extension, n is related to uniaxial straining in the x1- direction, and l is the associated cross modulus. The m and p are the transverse and longitudinal shear moduli. It is worth mentioning that in the micromechanical literature originating in the United Kingdom, the ﬁbers are often aligned with the xA Á x3 direction. That notation was frequently used in papers by Hill, Laws, Walpole and Willis, cited later. On the other hand, xA Á x1 is prevalent in papers on ﬁbrous laminates. Of course, change of coordinates has no effect on the physical deﬁnitions of the Hill’s moduli, but it changes the position of ﬁrst and third rows and columns in the
- 19. 2.3 Transversely Isotropic Composite Materials 29 Mij and Lij matrices, and it needs to be carefully monitored to prevent errors in applications. Moreover, (2.3.2) and (2.3.3) are often written in the contracted tensorial notation, where the multipliers 2 are transferred from the shear strain components to the shear moduli in the compliance and stiffness matrices, such that values of the stress components are not affected. This is illustrated in (2.3.11) and (2.3.13) below. For isotropic solids, Hill’s moduli appearing in the stiffness matrix (2.3.3) are expressed in bulk and shear moduli K and G and by Poisson’s ratio , according to k C m D n D 2G.1 / 1 2 k m D l D 2G 1 2 m D p D G k D K C G=3 l D K 2G=3 n D K C 4G=3 9 >= >; (2.3.6) If Lam´e constants and in (2.2.22a) are preferred, their connections to Hill’s moduli are k C m D n D C 2 k m D l D m D p D (2.3.7) It is often advantageous to separate the axisymmetric from the shear strain and stress components, and write the elastic constitutive relations (2.3.3) of transversely isotropic solids, for xA Á x1, as Ä 11 . 22 C 33/=2 D Ä n l l k Ä "11 ."22 C "33/ . 22 33/ D 2m."22 "33/ 23 D 2m"23 31 D 2p"31 12 D 2p"12 Ä "11 ."22 C "33/ D 1 .kn l2/ Ä k l l n Ä 11 . 22 C 33/=2 9 >>>>>>>>>>= >>>>>>>>>>; (2.3.8) Of course, elastic properties of actual ﬁbrous plies may not conform exactly to the widely used assumption of transverse isotropy, because the ﬁbers may not be uniformly distributed in the transverse plane. For example, plies reinforced by aramid, carbon or glass ﬁber tows, containing thousands of very thin ( 10 m) ﬁlaments, are often subdivided into ﬁber and matrix-rich regions. Also, certain metal and ceramic matrix plies are reinforced by monolayers of relatively thick ( 150 m) boron or silicon carbide ﬁbers. Such plies may have an orthotropic sym- metry on the macroscale. Evaluation of the nine engineering moduli of orthotropic solids would expand Table 2.4 and require six applied stress components. However, since the constants are usually measured in plane stress applied to thin ply layers, experimental results are limited to those appearing in the table, and deviations from transverse isotropy are neglected. Transversely isotropic material symmetry is also adopted for properties of some cylindrically anisotropic ﬁbers and of homogenized layered solids, such as surface coatings and thin ﬁlms.
- 20. 30 2 Anisotropic Elastic Solids As shown in Sect. 3.9, the microstructure of aligned ﬁber materials allows derivation of universal connections involving the overall moduli, and known phase moduli and volume fractions. In transversely isotropic ﬁber systems, the number of independent overall moduli is thereby reduced from ﬁve to three, the two shear moduli m and p, and one of the moduli k; l; n, such as k. However, it is often convenient to use all ﬁve moduli in derivations. 2.3.2 Walpole’s Notation Using again the xA Á x3 convention, Walpole (1969) writes the relation u D Aw between any symmetric second order tensors u; w, and a fourth-order tensor A, all expressed in the contracted tensorial notation, in the expanded form by Hill (1964) Ä .u11 C u22/=2 u33 D Ä ˛ ˇ1 ˇ2 Ä .w11 C w22/ w33 .u11 u22/ D 2ı.w11 w22/ u12 D 2ıw12 u23 D 2"w23 u31 D 2"w31 9 >>>>= >>>>; (2.3.9) For ˇ1 D ˇ2 D ˇ, the Aijkl D Aklij is diagonally symmetric and transversely isotropic with respect to xA Á x3. It is positive deﬁnite if and only if ˛ > 0; ı > 0; " > 0; and .˛ ˇ2 / > 0. In a symbolic form consistent with the contracted tensorial notation A D .2˛; ˇ; ; 2ı; 2"/ (2.3.10) Equations 2.3.9 can then be replaced by 2 6 6 6 6 6 6 6 6 6 4 u11 u22 u33 u23 u13 u12 3 7 7 7 7 7 7 7 7 7 5 D 2 6 6 6 6 6 6 6 6 6 4 .˛ C ı/ .˛ ı/ ˇ 0 0 0 .˛ ı/ .˛ C ı/ ˇ 0 0 0 ˇ ˇ 0 0 0 0 0 0 2" 0 0 0 0 0 0 2" 0 0 0 0 0 0 2ı 3 7 7 7 7 7 7 7 7 7 5 2 6 6 6 6 6 6 6 6 6 4 w11 w22 w33 w23 w13 w12 3 7 7 7 7 7 7 7 7 7 5 (2.3.11) The inverse w D A 1 u is written as A 1 D .ı=.2 /; ˇ=.2 /; ˛= ; 1=.2ı/; 1=.2"// (2.3.12)
- 21. 2.3 Transversely Isotropic Composite Materials 31 where D ˛ ˇ2 . In matrix form, w D A 1 u is 2 6 6 6 6 6 4 w11 w22 w33 w23 w13 w12 3 7 7 7 7 7 5 D 2 6 6 6 6 6 4 . = C 1=ı/=4 . = 1=ı/=4 ˇ=2 0 0 0 . = 1=ı/=4 . = C 1=ı/=4 ˇ=2 0 0 0 ˇ=2 ˇ=2 ˛= 0 0 0 0 0 0 1=.2"/ 0 0 0 0 0 0 1=.2"/ 0 0 0 0 0 0 1=.2ı/ 3 7 7 7 7 7 5 2 6 6 6 6 6 4 u11 u22 u33 u23 u13 u12 3 7 7 7 7 7 5 (2.3.13) Walpole’s notation is often used to describe different diagonally symmetric and transversely isotropic tensors in the micromechanics literature. Notice that the symbolic forms (2.3.10) and (2.3.12) are not affected by the choice of direction of the axis xA of rotational symmetry; however, appropriate exchanges of rows and columns are required in the matrices (2.3.11) and (2.3.13). Moreover, notice that in the uij and wij in (2.3.9) are usually regarded as coefﬁcients of the stress and strain tensors, hence the tensorial shear strain components in (2.3.11) and (2.3.13) are "23 D w23, etc., in contrast to their engineering form 2"23 D w23, etc. The engineering and contracted tensorial matrix notations invite the connections D L" D LEG"EG LEG D L 1 D 1 L " D 1 "EG D M D 1 MEG MEG D M D M ) [1.1.22] where the diagonal matrix D diag.1; 1; 1; 2; 2; 2/. However, to preserve diagonal symmetry of the stiffness or compliance matrices L; M, these connections apply only to orthotropic, tetragonal, transversely isotropic, cubic and isotropic solids, all free of coupling between normal and shear strains and stresses. Examples of application of Walpole’s notation include stiffness and compliance matrices of transversely isotropic solids, written in the symbolic form consistent with the contracted tensorial notation and the xA Á x3 convention as L D .2k; l; n; 2m; 2p/ M D .n=.2kE/; l=.2kE/; 1=E; 1=2m; 1=2p/ (2.3.14) For xA Á x1, the corresponding L and M matrices in the engineering notation are given by (2.3.3) and (2.3.2), where kE D kE11 D kn l2 . Of course, (2.3.14) could be converted to engineering notation by changing 2m; 2p to m; p: For cubic material symmetry of §2.2.7, the stiffness and compliance can be written as L D .3Ä; 2 ; 2 0 / M D Œ1=.3Ä/; 1=.2 /; 1= .2 0 / (2.3.15) in terms of Zener’s moduli (2.2.18). For isotropic stiffness and compliance tensors, the original Hill’s (1965a) notation is, as in (2.2.29) L D .3K; 2G/ M D .1=.3K/; 1=.2G// (2.3.16)
- 22. 32 2 Anisotropic Elastic Solids Forms similar to M are also be used to deﬁne other tensors that have the dimension of a compliance, such as the P tensor in Sect. 4.6. 2.4 Cylindrically Orthotropic Materials This is a separate symmetry class, characterized by distinct elastic moduli which are constant along each of the radial, tangential or hoop, and axial or longitudinal directions of cylindrical coordinates r; ™; z. An orthogonal transformation from the Cartesian to the cylindrical system of coordinates is described by fr ; ™; zgT i D aijxj (2.4.1) where the aij is given in (2.2.5). Invariance is preserved only under translation in the z-direction and under a rotation by ™. Nine stiffness coefﬁcients describe this type of symmetry. The constitutive relation uses the stiffness matrix C, and is typically written as 2 6 6 6 6 6 6 6 4 rr zz z zr r 3 7 7 7 7 7 7 7 5 D 2 6 6 6 6 6 6 6 4 Crr Cr Crz 0 0 0 C C z 0 0 0 Czz 0 0 0 G z 0 0 sym: Gzr 0 Gr 3 7 7 7 7 7 7 7 5 2 6 6 6 6 6 6 6 4 "rr " "zz 2" z 2"zr 2"r 3 7 7 7 7 7 7 7 5 (2.4.2) Radially or circumferentially orthotropic materials satisfy Crr > C or Crr < C , respectively. Note that a transformation inverse to (2.4.1) renders the stiffness coefﬁcients dependent on the angle ™, and thus on position in the Cartesian coordinate system. Cylindrical orthotropic symmetry applies to ﬁber coatings or laminated com- posite cylinders, and also to anisotropic ﬁbers where reliable experimental data are typically available only for the Czz coefﬁcient. Therefore, such ﬁbers are often assumed to be only transversely isotropic, so that their properties can be extracted by micromechanical methods from those measured on matrix-based composites. The number of independent coefﬁcients is then reduced from nine to ﬁve, using the following connections with Hill’s moduli, written here for the x3 Á z-axis of rotational symmetry Crr D C D k C m Cr D k m Crz D C z D l Czz D n Crr Cr D 2Gr Gr D m G z D Gzr D p ) (2.4.3)
- 23. 2.5 Young’s Modulus, Shear Modulus and Poisson’s Ratio 33 2.5 Young’s Modulus, Shear Modulus and Poisson’s Ratio Restrictions imposed on the elastic constants by positive deﬁniteness of the strain energy function allow directional dependence of elastic moduli of anisotropic solids and thus invite search for directions that correspond to extremal values of engineering constants of practical interest, such as Young’s modulus, shear modulus, and Poisson’s ratio. As pointed out by Hayes and Shuvalov (1998), Sirotin and Shakol’skaya (1982) had derived the following expressions of the three moduli of any anisotropic elastic solid, as functions of compliance coefﬁcients and spatial directions. In particular, the Young’s modulus E .n/, deﬁned as the ratio of the normal stress to normal strain, both acting in the direction of a certain unit vector n, is given by E.n/ D 1=.Mijklni nj nknl / (2.5.1) Explicit expressions and graphs of E .n/ for materials of different symmetry classes can be found in Backus (1970) and Nye (1957, 1985). The shear modulus G.m; n/ is deﬁned as the ratio of the shear stress to the shear strain on a square element whose two sides are described by two orthogonal unit normal vectors m and n; such that n n D m m D 1 and m n D 0. G.m; n/ D G.n; m/ D 1=.4Mijklni mj nkml/ (2.5.2) The Poisson’s ratio .m; n/ is deﬁned as the negative transverse strain along m, divided by the axial strain in the direction of stretching force along the direction n. .m; n/ D Mijklmi mj nknl ı .Mpqrsnpnqnr ns / (2.5.3) Ting (2005a) studied the maximum, minimum and saddle points of Young’s mod- ulus for a general anisotropic elastic material. He also shows that certain orthotropic and hexagonal materials can have a Young’s modulus that is independent of the direction n (Ting 2005b). Srinivasan and Nigam (1969) derived certain invariant elastic moduli for crystals. Hayes and Shuvalov (1998) derived connections between extreme values of the three moduli of cubic materials, which had been identiﬁed by Turley and Sines (1971). Li (1976) presented a method for calculating Young’s modulus, shear modulus and Poisson’s ratio for hexagonal materials. It turns out that (2.5.3) imposes no limits on the extreme values of Poisson’s ratio in all anisotropic materials, where it may reach an arbitrarily large positive or negative value for certain directions of the above vectors (Boulanger and Hayes 1998; Ting 2004; Ting and Chen 2005; Ting and Barnett 2005). This admits existence and suggests design of auxetic materials with negative Poison’s ratios (Lakes 1993; Zheng and Chen 2001; Baughman et al. 1998). They expand when stretched, which may enhance their shear moduli, indentation resistance and fracture toughness (Lakes 1987, 2000). With few exceptions, they do not exist in nature.
- 24. 34 2 Anisotropic Elastic Solids Table 2.5 Selected Symbols 0 Volume of the comparison medium surrounding r 0 r Volume of homogeneous inclusion or inhomogeneity Total volume D 0 C r @ Surface of volume @ r Interface between r and 0 V, Vr, cr D Vr/ V Total and inhomogeneity volumes, and phase volume fraction in a composite aggregate @Vr Interface between inhomogeneity Lr in Vr and matrix L1 L0, M0 Stiffness and compliance of a comparison medium in 0 L1, M1 Stiffness and compliance of the matrix phase Lr, Mr Stiffness and compliance of an inhomogeneity in r or Vr L, M Overall stiffness and compliance of a composite aggregate "0 ; "0 Uniform overall strain applied to or V 0, r Uniform eigenstrain applied in 0, and r or Vr N ; N Overall stress caused in or V by the load set f"0 ; r ; 0g N Overall eigenstress caused in and V by the load set f"0 ; r ; 0g 0 ; 0 Uniform overall stress applied to or V 0, r Uniform eigenstress applied in 0 and r or Vr N" ; N" Overall strain caused by load set f 0 ; r ; 0 g in or V N Overall eigenstrain caused by load set f 0 ; r ; 0 g "r ; N"r Uniform and average local strain in r or Vr r ; N r Uniform and average local stress in r or Vr eq r ; eq r Uniform equivalent eigenstrain and eigenstress in r or Vr dq r ; dq r Uniform damage-equivalent eigenstrain and eigenstress in r or Vr Tr, Rrr, Rr0 Partial strain and eigenstrain concentration factors Wr, Nrr, Nr0 Partial stress and eigenstress concentration factors However, they can be realized by certain symmetric laminates with . ˙ ™/S layups, Sect. 10.7, or by homogenization of speciﬁc microstructures. For example, Almgren (1985) designed structures, in two or three dimensions consisting of rods, hinges, and springs that have a negative Poisson’s ratio. Foam materials with negative Poisson’s ratio have also been developed (Lakes 1987). Evans et al. (1991) used molecular modeling techniques to design a molecular network with a negative Poisson’s ratio (see also Guo and Wheeler 2006). Some potential applications of auxetic materials can be found in review articles by Evans (1991) and Lakes (1993). A list of symbols frequently used in the chapters that follow appears in Table 2.5.

No public clipboards found for this slide

×
### Save the most important slides with Clipping

Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.

Be the first to comment